A Bamboo-Inspired Nanostructure Design for Flexible, Foldable, and Twistable Energy Storage Devices Yongming Sun,†,‡ Ryan B. Sills,§,∥ Xianluo Hu,*,† Zhi Wei Seh,‡ Xu Xiao,⊥ Henghui Xu,† Wei Luo,† Huanyu Jin,⊥ Ying Xin,# Tianqi Li,⊥ Zhaoliang Zhang,# Jun Zhou,⊥ Wei Cai,§ Yunhui Huang,*,† and Yi Cui*,‡,○ †
State Key Laboratory of Materials Processing and Die & Mold Technology, School of Materials Science and Engineering and Wuhan National Laboratory for Optoelectronics (WNLO), and College of Optoelectronic Science and Engineering, Huazhong University of Science and Technology, Wuhan 430074, P. R. China ‡ Department of Materials Science and Engineering and §Department of Mechanical Engineering, Stanford University, Stanford, California 94305, United States ∥ Sandia National Laboratories, Livermore, California 94551, United States # School of Chemistry and Chemical Engineering, University of Jinan, Jinan 250022, P. R. China ○ Stanford Institute for Materials and Energy Sciences, SLAC National Accelerator Laboratory, 2575 Sand Hill Road, Menlo Park, California 94025, United States ⊥
S Supporting Information *
ABSTRACT: Flexible energy storage devices are critical components for emerging ﬂexible electronics. Electrode design is key in the development of all-solid-state supercapacitors with superior electrochemical performances and mechanical durability. Herein, we propose a bamboo-like graphitic carbon nanoﬁber with a well-balanced macro-, meso-, and microporosity, enabling excellent mechanical ﬂexibility, foldability, and electrochemical performances. Our design is inspired by the structure of bamboos, where a periodic distribution of interior holes along the length and graded pore structure at the cross section not only enhance their stability under diﬀerent mechanical deformation conditions but also provide a high surface area accessible to the electrolyte and low ion-transport resistance. The prepared nanoﬁber network electrode recovers its initial state easily after 3-folded manipulation. The mechanically robust membrane is explored as a free-standing electrode for a ﬂexible all-solid-state supercapacitor. Without the need for extra support, the volumetric energy and power densities based on the whole device are greatly improved compared to the state-of-the-art devices. Even under continuous dynamic operations of forceful bending (90°) and twisting (180°), the as-designed device still exhibits stable electrochemical performances with 100% capacitance retention. Such a unique supercapacitor holds great promise for high-performance ﬂexible electronics. KEYWORDS: Bamboo-like carbon nanoﬁbers, mechanical properties, supercapacitor, electrochemical performances been made in the design of graphene-based ﬁlm electrodes for all-solid-state supercapacitors.1,13,14 Carbon nanotube architectures have also been successfully designed as mechanical support to develop ﬁber type supercapacitors with superior mechanical durability.3,15,16 In spite of this progress, the energy density of the devices is still limited by the use of ﬂexible but inert substrates or the large proportion of the low-speciﬁccapacitance carbon nanotubes. In other words, an ideal electrode material for ﬂexible all-solid-state supercapacitors should possess high speciﬁc capacitance and be highly ﬂexible by itself without the need for mechanical support. However, to date, there are very few successful examples of such all-solid-
lexible electronics is aimed to be portable, lightweight, bendable, foldable, twistable, and even wearable. Due to these features, the corresponding power sources should be lightweight and stable under diﬀerent mechanical deformation conditions. Recently, much progress has been made in the development of ﬂexible all-solid-state supercapacitors for ﬂexible electronics owing to their ease of handing, small size, and safety.1−7 The main limitations, however, are their low volumetric energy density and limited mechanical durability.8−12 A typical fabrication procedure of an all-solid-state supercapacitor includes the synthesis of active materials on a conductive and ﬂexible substrate, followed by assembly into devices using a gel electrolyte. However, little emphasis has been placed on the development of free-standing ﬂexible active materials without the need for extra support, which is vital for the improvement of energy and power densities based on the volume of the whole devices. In this respect, some progress has © XXXX American Chemical Society
Received: February 24, 2015 Revised: April 15, 2015
DOI: 10.1021/acs.nanolett.5b00738 Nano Lett. XXXX, XXX, XXX−XXX
Figure 1. Schematic of the bamboo-inspired nanostructure design and three-point bending simulations. (a) The graded structure of bamboos. (b) Schematic of the bamboo-inspired nanostructure design. (c) Results from three-point bending simulations of diﬀerent ﬁber geometries: solid ﬁber, tube, bamboo-like ﬁber with hollow cores (Bamboo), and fully porous bamboo-like ﬁber with both hollow cores and graded pores through the cross section (Bamboo, 0.04 E). (Left) The force−displacement response of the nanoﬁbers (F is the force, E is Young’s modulus, r0 is the outer radius). (Right) Snapshots of the deformation and von Mises stress distribution (normalized by the Young’s modulus) at vertical displacements of v/r0 = 10 (v is the vertical displacement). The simulation results indicate that bamboo-like nanoﬁbers have much better mechanical durability and ﬂexibility than the solid ﬁbers and tubes.
global elastic modulus of the nanoﬁbers, the parameter that controls the deformation response to loading over length scales much larger than the micro/mesopore diameters, to approximately 4% of the base material’s value (Supporting Information, Method S1). This reduction in the global modulus results in an overall reduction in stiﬀness of the nanoﬁbers, making the load required to sustain the same amount of deformation about a factor of 20 lower. Second, the macropores that give the nanoﬁbers their bamboo-like hollow cores also act to reduce the stiﬀness both globally, by lowering the overall moment of inertia, and locally, by providing thin, ﬂexible regions at the walls of the pores. Additionally, the reinforcement provided by the webs of material separating the macropores give the bamboo-like nanoﬁbers the important property of robustness against localized deformation. To demonstrate this eﬀect, a series of three-point bending simulations were conducted for a solid ﬁber, a bamboo-like ﬁber, and a tubular ﬁber of equivalent moment of inertia to the bamboo-like ﬁber (Figure 1c, Supporting Information, Method S2). Clearly the stiﬀnesses of the bamboo-like and tubular ﬁbers are reduced relative to the solid ﬁber. Additionally, we see that in the case of the tubular ﬁber, the deformation becomes highly localized as the tube “crimps” together. In contrast, the bamboo-like ﬁber maintains the same cross-sectional form at the site of loading, indicating it is much more robust. Hence, we believe the bamboo-like ﬁbers are much better at sharing/ shedding load in the 2D webs comprising the supercapacitors without inducing localized failure.
state supercapacitors showing stable electrochemical performances under continuous dynamic mechanical deformation conditions. Bamboo is a representative example of plants that possess superior ﬂexibility and mechanical durability. Its geometry consists of a functionally graded structure from macroscopic scale to microscopic scale that is adapted to withstand the forces of nature: The “nodes” provide additional reinforcement for the “culm”, preventing buckling due to bending and axial cracks. The graded structure of the ﬁbers through their crosssection accommodates the stress distribution due to a bending moment and thus optimizes the ﬂexural properties (Figure 1a).17−19 Here, inspired by the structure of bamboo, we demonstrate a novel, multiscale, hierarchical carbon nanostructure. Such a design has the following characteristics: 1D graphitic carbon nanoﬁbers with uniform discontinuous hollow interiors (macropores) as well as graded nanopores (mesopores and micropores) through the cross-section of the nanoﬁbers (Figure 1b). These hierarchical and well-balanced macro-, meso- and microporosities help to provide a high ion-accessible surface area and low ion transport resistance, which are the keys to achieving high speciﬁc capacitance and rate capability in electrical double-layer capacitors.20−24 Meanwhile, superior mechanical durability and ﬂexibility can also be expected in terms of the unique pore structure. The micro/mesopores account for 79% of the porosity (based on high-resolution nitrogen-sorption analyses discussed later). According to theoretical25 and empirical26 estimates, they act to reduce the B
DOI: 10.1021/acs.nanolett.5b00738 Nano Lett. XXXX, XXX, XXX−XXX
Figure 2. Fabrication and characterization of the bamboo-like carbon nanoﬁbers. (a) Schematic of the fabrication process of the bamboo-like carbon nanoﬁbers. TEOS/PAN composite nanoﬁbers were ﬁrst prepared by electrospinning. By heating the precursors at 1200 °C in a H2/Ar (5/95 in volume) atmosphere, ultraﬁne SiO2 clusters transfer and aggregate into much larger SiO2 particles uniformly lined in the core region within the nanoﬁbers, while their transfer path forms interconnected and graded meso/micropores. The bamboo-like nanoﬁbers are ﬁnally obtained after removing the SiO2 particles in a HF aqueous solution. (b,c,d) TEM images of the initial TEOS/PAN composite nanoﬁbers (b), SiO2/carbon composite nanoﬁbers (c) and bamboo-like carbon nanoﬁbers (d). The circles in (c) show the existence of SiO2 particles in the core of the SiO2/ carbon composite nanoﬁbers. (e,f,g) SEM images (e,f) and HRTEM image (g) of the as-prepared carbon nanoﬁbers.
interconnect with each other, forming a tight 2D web with submicron/micron size interﬁber porosity (Figure 2f). The pore-size distribution, pore volume, and speciﬁc surface area (SSA) of the carbon nanoﬁbers were studied using highresolution nitrogen-sorption experiments with advanced methods based on density functional theory (DFT) (Supporting Information, Figure S5). The bamboo-like carbon nanoﬁbers have a continuous pore-size distribution from 0.64 nm to over 100 nm. Their SSA is as high as ∼1912 m2 g−1, and their pore volume is ∼2.27 cm3 g−1. Furthermore, their porosity and SSA can be tuned easily by controlling the diﬀusion of the SiO2 clusters in the ﬁbers (Supporting Information, Figures S6 and S7), indicating great versatility in manipulating the pore structure. A high resolution transmission electron microscopy (HRTEM) image shows that the shells of these bamboo-like carbon nanoﬁbers consist of interconnected and highly curved graphitic carbon nanosheets, supporting their superior structural ﬂexibility and electrical conductivity (Figure 2g). Detailed structure characterization, including electron energy loss spectroscopy (EELS), powder X-ray diﬀraction (XRD), X-ray photoelectron spectroscopy (XPS), elemental analysis, and Raman spectroscopy (Supporting Information, Figures S8− S11), further conﬁrm their graphitic carbon structure. Due to the bamboo-like ﬁber structure and tight organization of the 2D ﬁbrous felts, our carbon nanoﬁber network electrode is ﬂexible, foldable, and pliable. The prepared carbon
The schematic of the fabrication process of the bamboo-like carbon nanoﬁbers is shown in Figure 2a. In a typical procedure, a precursor of polyacrylonitrile (PAN) and tetraethyl orthosilicate (TEOS) in dimethylformamide (DMF) was made into a white nanoﬁber web by electrospinning (Supporting Information, Figures S1 and S2). Black carbon nanoﬁber network electrodes were then obtained after thermal treatment of these TEOS/PAN nanoﬁber webs in a H2/Ar (5/ 95 in volume) atmosphere followed by etching SiO2 in an aqueous HF solution (Supporting Information, Figure S3). The SiO2 molecular clusters are very uniformly distributed within the as-electrospun nanoﬁbers (Figure 2b). In the heat treatment process, these ultraﬁne SiO2 clusters transfer inward and aggregate into much larger SiO2 particles (tens of nanometers in size) in the center of the nanoﬁbers (Figure 2c, Supporting Information, Figure S4), while their transfer path forms a graded and interconnected pore structure within the shell of the hybrid nanoﬁbers, accompanied by the carbonization of PAN. Etching these SiO2 particles generates a sequence of spherical holes uniformly distributed along the axes of the nanoﬁbers (Figure 2d). These hollow interiors, together with a graded and interconnected pore structure: small micro/mesopores in the outer surface and larger mesopores in the inner region of the shell (Figure 2e), endow the assynthesized carbon nanoﬁbers with a unique porous architecture. Meanwhile, these bamboo-like carbon nanoﬁbers C
DOI: 10.1021/acs.nanolett.5b00738 Nano Lett. XXXX, XXX, XXX−XXX
Information, Movie S2), and a ﬂat cross-section was observed (Figure 3g), indicating a brittle fracture process. Here, the capacitive properties of the bamboo-like carbon nanoﬁber webs were explored by using a traditional threeelectrode conﬁguration in a liquid electrolyte (Figure 4). Figure 4a and b shows the typical cyclic voltammetry (CV) curves at various scan rates between 10 and 2000 mV s−1, within the potential range of −0.9 to 0 V (vs Hg/HgO). Rectangular shapes of the CVs are obtained even at a very high scan rate of 2000 mV s−1, indicating a very fast and eﬃcient charge transfer. Figure 4c shows the nearly triangular shape of the galvanostatic charge/discharge curves obtained at a high current density of 100 A g−1, suggesting the formation of eﬃcient electrochemical double layers and fast ion transport within the carbon nanoﬁber electrodes. The as-made carbon nanoﬁber electrodes exhibit an outstanding speciﬁc capacitance as high as 236 F g−1 at a current density of 5 A g−1 and show a very small decrease in gravimetric capacitance even at very high current densities (∼30% at 100 A g−1) (Figure 4c and d). Meanwhile, the electrodes also display an extraordinarily high stability with ∼100% of the initial capacitance after 5000 cycles tested at a constant current density of 10 A g−1 (Figure 4e). Our bamboolike carbon nanoﬁber web, possessing inherent 3D interconnected hierarchical porous structures with high SSA, evidently supports its potential applications for high-performance supercapacitors. The large and accessible SSA to the electrolyte enables high speciﬁc capacitance. The superior rate capability can be ascribed to the highly conductive pathway for electrons and fast transport channels for ions. Previous studies indicated that the power characteristics of many carbon materials remains limited due to an intrinsically high fraction of microporosity, which in turn limits pore accessibility of the electrolyte ions at high current densities.27 Here, our bamboo-like porous carbon nanoarchitecture is successful in achieving high power density as well as keeping high energy density by creating facile electron/ion-transport pathways. With the combination of superior electrochemical properties and mechanical durability, the bamboo-like carbon nanoﬁber webs are promising candidates for ﬂexible all-solid-state supercapacitor electrodes. To explore the electrochemical performances of the assynthesized bamboo-like carbon nanoﬁber webs as all-solidstate supercapacitor electrodes, symmetric supercapacitors can be readily made by sandwiching a cellulose separator between two identical carbon nanoﬁber web electrodes. The freestanding carbon nanoﬁber webs serve as both the active material and current collector in the two-electrode cell conﬁguration because of their good conductivity. Moreover, the as-made devices do not require any ﬂexible substrates (e.g., polyethylene terephthalate substrate, conductive aluminum foil, and nitrocellulose membrane) due to the superior mechanical durability of the bamboo-like carbon nanoﬁber webs. The thickness of devices is tunable by selecting carbon nanoﬁber webs with diﬀerent thicknesses, making them potentially useful in microdevice applications.28 It has been recognized that supercapacitor electrodes comprising of an active material coating layer on ﬂexible conductive support (e.g., a carbon cloth) and an active thin ﬁlm on a ﬂexible substrate (e.g., polyethylene terephthalate) usually have a smaller internal resistance and better ion diﬀusion characteristics to achieve a higher apparent speciﬁc capacitance when normalized by the weight of the active materials. However, high energy and power densities cannot always be obtained on the basis of the total volume or weight of the devices due to the presence of inactive
membrane recovers its initial state easily after 3-folded manipulation, indicating its excellent mechanical durability (Figure 3a, Supporting Information, Movie S1). Figure 3b
Figure 3. Mechanical properties and structural characterizations of the as-obtained bamboo-like carbon nanoﬁber webs. (a) A piece of carbon nanoﬁber web is 3-folded and recovers its initial state easily, indicating its excellent mechanical durability. More detailed information on the mechanical durability of the as-prepared bamboo-like carbon nanoﬁber webs under dynamic forceful operations can be seen in Supplementary Movie 1. (b) SEM images of a piece of carbon nanoﬁber web with a bending angle of 180°. (c,d) TEM images of carbon nanoﬁbers from a membrane that is folded (180°), twisted (180°), extruded, and sandwiched between two TEM grids (c) and their recover after the release of strain (d). (e) TEM image of a damaged bamboo-like carbon nanoﬁber, which retains connected remnants. (f) Digital picture of a membrane of solid ﬁbers failed under a small bending angle (